E ﬀ ect of Processing Technique Factors on Structure and Photophysical Properties of Perovskite Absorption Layer by Using Two-Step Spin-Coating Method

: The investigation of crystal growth is crucial for us to improve the ﬁlm quality and photophysical properties of CH 3 NH 3 PbI 3 (MAPbI 3 ). In the two-step spin-coating process, the crystal structure could be modulated by controlling the growth conditions of PbI 2 and CH 3 NH 3 I (MAI) layers. In this paper, the PbI 2 layer was treated with annealing under di ﬀ erent times. A liquid–liquid di ﬀ usion (LLD) mechanism is proposed to modify the deposition of MAI precursor solution and enhance the ﬂatness of organic–inorganic hybrid perovskite ﬁlm. Furthermore, the perovskite ﬁlms are prepared using di ﬀ erent concentrations of MAI. The evolution process of perovskite structure is observed by modulating the concentration of MAI. The spin-coating of moderate MAI tends to form high quality MAPbI 3 ﬁlms with enhanced absorption and carrier extraction capabilities. The high concentration of MAI would cause the perovskite phase transition, which provides a novel perspective to modulate the structure of organic–inorganic hybrid perovskite in the two-step spin-coating process, although it deteriorates the device performance. on the quality of organic–inorganic hybrid perovskite ﬁlm was investigated. We found the LLD of MAI solution and unannealed PbI 2 layer was conducive to forming ﬁlms with ﬂat coverage, and the rough ﬁlm was obtained with liquid–solid di ﬀ usion (LSD). Then, concentration of the MAI solution was adjusted to investigate the morphology and the photophysical properties of various organic–inorganic hybrid perovskite layers. Di ﬀ erent from previous researches, the high concentration of MAI was adopted. It could be observed that the PbI 2 grain crystals formed at the interface between the perovskite were annealed on a hot plate at 150 ◦ C for 15 min. All experiments were performed at room temperature in ambient condition.


Introduction
The past ten years have witnessed the rapid development of perovskite solar cells (PSCs) [1][2][3][4]. The perovskite material, as the light absorption layer of the solar cells, has received tremendous attention, due to its suitable band gap [5][6][7], long charge carrier diffusion lengths [8][9][10], and good light absorption capability [11]. Therefore, the preparation process for the perovskite layer plays a crucial role in the performance of solar cell devices [12].

Cleaning of FTO Conductive Glass
First, a mixture solution of detergent and deionized water was added to the Petri dish, and the FTO glass substrate was dipped in the solution for ten min. The purpose is to remove impurities and grease on the surface of the substrate, which would improve the conductivity of the substrate. Then we placed the cleaned FTO substrate glass in a Petri dish with the conductive surface facing up. Detergent solution (volume ratio: acetone:isopropanol:deionized water = 1:1:1) was added to the Petri dish. Then, the Petri dish was placed in an ultrasonic cleaner to clean for 20 min. Ethanol was used to clean the FTO, according to the above method. Lastly, the dried FTO glass substrate was placed in the drawer type UV light cleaning machine, and treated with ultraviolet ozone for 15 min to eliminate organic impurities and improve its hydrophilicity.

Preparation of NiO x Hole Transport Layer
NiO solution was stirred by temperature-control magnetic stirrer for 8 h. Then, the filtered solution was spin-coated on an FTO substrate at 4000 rpm for 30 s. Finally, the FTO/NiO x substrate was annealed on a hot plate at 150 • C for 10 min, and the as-annealed NiO x film was sintered at 350 • C for 1 h in a ceramic fiber muffle furnace (the rising time was set to be half an hour).

Preparation of Perovskite Thin Film
The experiment was divided into two sections. In the first part of the experiment, 0.5993 g (1.3 mmol) PbI 2 powder was dissolved into a mixture solution of DMSO and DMF (1 mL, volume ratio: 0.05:0.95) completely, and spin-coated on an FTO/NiO x substrate at 1500 rpm for 30 s. Then, the FTO/NiO x /PbI 2 samples were annealed on a hot plate at different times (0 s, 10 s, and 20 s), and the annealing temperature was 150 • C. Finally, 73 mg of MAI powder was dissolved in isopropanol solution (1 mL) completely, and spin-coated onto the PbI 2 film at 1500 rpm for 30 s. The formed films were annealed on a hot plate at 150 • C for 150 min. The annealing time of the PbI 2 layer (0 s) was selected in Section 2 of our experiment. The different weights of MAI powder (53 mg, 73 mg, and 93 mg) were dissolved in isopropanol solution (1 mL) completely, and spin-coated onto the PbI 2 film at 1500 rpm for 30 s. Then, the films were annealed on a hot plate at 150 • C for 15 min. All experiments were performed at room temperature in ambient condition.

Characterization
The morphology of organic-inorganic hybrid perovskite film was measured with a scanning electron microscope (SEM) (SIGMA, Zeiss, Jena, Germany). X-ray diffraction (XRD) data of perovskite layers deposited on FTO/NiO x bottoms were measured with an X-ray diffractometer (D8 Focus, Bruker, Dresden, Germany). Absorption spectra of the perovskite films on FTO/NiO x bottoms were measured with an ultraviolet-visible (UV-Vis) absorption spectrometer (Avantes, Apeldoom, The Netherlands), and a LabRAW HR800 photoluminescence (PL) testing system (HORIBA Jobin Yvon, Paris, France) was employed to obtain the photoluminescence (PL) spectroscopy data.

Results and Discussion
In the two-step preparation process, the various annealing times of the PbI 2 layer are investigated firstly. In our work, the coated PbI 2 layers were annealed for 0 s, 10 s, and 20 s, respectively. To ensure the reliability of the experiment, the MAI concentration of 73 mg/mL was selected. SEM images and enlarged images of perovskite films with different PbI 2 annealing times are shown in Figure 1. The unannealed condition of coated PbI 2 results in the retention of DMSO and DMF solution, which is conducive to the diffusion of MAI precursor solution. Therefore, the perovskite films with high surface flatness and denseness are obtained through liquid-liquid diffusion (Figure 1a,d). The increase in annealing time leads to the growth of PbI 2 solid, which reacts with deposited MAI solution to form organic-inorganic hybrid perovskite film with loose structure in the surface. Thin films with rough surface and a few voids are formed through two diffusion mechanisms (liquid-liquid and liquid-solid), as shown in Figure 1b,c,e,f. Crystals 2020, 10, x FOR PEER REVIEW 4 of 12 mg) were dissolved in isopropanol solution (1 mL) completely, and spin-coated onto the PbI2 film at 1500 rpm for 30 s. Then, the films were annealed on a hot plate at 150 °C for 15 min. All experiments were performed at room temperature in ambient condition.

Characterization
The morphology of organic-inorganic hybrid perovskite film was measured with a scanning electron microscope (SEM) (SIGMA, Zeiss, Jena, Germany). X-ray diffraction (XRD) data of perovskite layers deposited on FTO/NiOx bottoms were measured with an X-ray diffractometer (D8 Focus, Bruker, Dresden, Germany). Absorption spectra of the perovskite films on FTO/NiOx bottoms were measured with an ultraviolet-visible (UV-Vis) absorption spectrometer (Avantes, Apeldoom, The Netherlands), and a LabRAW HR800 photoluminescence (PL) testing system (HORIBA Jobin Yvon, Paris, France) was employed to obtain the photoluminescence (PL) spectroscopy data.

Results and Discussion
In the two-step preparation process, the various annealing times of the PbI2 layer are investigated firstly. In our work, the coated PbI2 layers were annealed for 0 s, 10 s, and 20 s, respectively. To ensure the reliability of the experiment, the MAI concentration of 73 mg/mL was selected. SEM images and enlarged images of perovskite films with different PbI2 annealing times are shown in Figure 1. The unannealed condition of coated PbI2 results in the retention of DMSO and DMF solution, which is conducive to the diffusion of MAI precursor solution. Therefore, the perovskite films with high surface flatness and denseness are obtained through liquid-liquid diffusion (Figure 1a,d). The increase in annealing time leads to the growth of PbI2 solid, which reacts with deposited MAI solution to form organic-inorganic hybrid perovskite film with loose structure in the surface. Thin films with rough surface and a few voids are formed through two diffusion mechanisms (liquid-liquid and liquid-solid), as shown in Figure 1b,c,e,f. SEM cross-section views of organic-inorganic hybrid perovskite thin films prepared with 0 s, 10 s, and 20 s annealing time of PbI2 layers are shown in Figure 2. With 0 s annealing of PbI2, the interface of perovskite film and hole transport layer is flat with even coverage (Figure 2a). As the annealing time increases, the growth of irregular crystals can be observed at the interface (Figure 2b), resulting in the decrease in film flatness and thickness. More serious deterioration at the interface is shown in Figure 2c, which would lead to the increase in defect density. Overall, the poor interfaces of 10 s and 20 s annealing samples are due to the growth of PbI2 crystals and loose structure formed through SEM cross-section views of organic-inorganic hybrid perovskite thin films prepared with 0 s, 10 s, and 20 s annealing time of PbI 2 layers are shown in Figure 2. With 0 s annealing of PbI 2 , the interface of perovskite film and hole transport layer is flat with even coverage (Figure 2a). As the annealing time increases, the growth of irregular crystals can be observed at the interface (Figure 2b), resulting in the decrease in film flatness and thickness. More serious deterioration at the interface is shown in Figure 2c, which would lead to the increase in defect density. Overall, the poor interfaces of 10 s and 20 s annealing samples are due to the growth of PbI 2 crystals and loose structure formed through liquid-solid diffusion. Through the analysis of the morphology, it can be found that the annealing time  To illustrate the growth of perovskite films in detail, the evolution process of organic-inorganic hybrid perovskite films with different annealing conditions is shown in Figure 3. With 0 s annealing, DMF and DMSO solution is not completely volatilized. The contact between the MAI precursor solution (73 mg/mL) and the PbI2 solution belongs to a liquid-liquid diffusion. It is easier for MAI solution to diffuse into the bottom layer, which is conducive to growing flat film. However, part of a solid PbI2 crystal is formed on the topmost layer of the PbI2 film with the annealing condition. With the deposition of MAI precursor solution, loose and uneven perovskite film is partially formed through liquid-solid diffusion (LSD) between precursor solution and the solid topmost layer of PbI2. Therefore, the rough film is obtained, as shown in Figure 3, which is ascribed to the different contact mechanism and crystal growth rate of LLD and LSD between the MAI precursor solution and the PbI2 layer. The adjustment of annealing mainly depends on the time and temperature. Studies have demonstrated that PbI2 film with high crystallinity can be obtained under annealing conditions of high temperature for several minutes, and the MAPbI3 film retains a similar trend. However, in our optimized processing, the compact and flat perovskite film is formed on the liquid PbI2 bottom layer. In the two-step method, the morphology and photophysical properties of the light-absorbing layer can be controlled by the MAI concentration [25]. It is pointed out that the grain size and surface roughness of the perovskite layer are related to the concentration of MAI. In this part of the experiment, different concentrations of MAI are introduced, and the PbI2 layer is not annealed, employing the previous optimization strategy. SEM top views and enlarged views of organic- To illustrate the growth of perovskite films in detail, the evolution process of organic-inorganic hybrid perovskite films with different annealing conditions is shown in Figure 3. With 0 s annealing, DMF and DMSO solution is not completely volatilized. The contact between the MAI precursor solution (73 mg/mL) and the PbI 2 solution belongs to a liquid-liquid diffusion. It is easier for MAI solution to diffuse into the bottom layer, which is conducive to growing flat film. However, part of a solid PbI 2 crystal is formed on the topmost layer of the PbI 2 film with the annealing condition. With the deposition of MAI precursor solution, loose and uneven perovskite film is partially formed through liquid-solid diffusion (LSD) between precursor solution and the solid topmost layer of PbI 2 . Therefore, the rough film is obtained, as shown in Figure 3, which is ascribed to the different contact mechanism and crystal growth rate of LLD and LSD between the MAI precursor solution and the PbI 2 layer. The adjustment of annealing mainly depends on the time and temperature. Studies have demonstrated that PbI 2 film with high crystallinity can be obtained under annealing conditions of high temperature for several minutes, and the MAPbI3 film retains a similar trend. However, in our optimized processing, the compact and flat perovskite film is formed on the liquid PbI 2 bottom layer.
Crystals 2020, 10, x FOR PEER REVIEW 5 of 12 liquid-solid diffusion. Through the analysis of the morphology, it can be found that the annealing time of the PbI2 layer has an effect on the surface flatness of the perovskite film. The result is similar to the previous report of our group. To illustrate the growth of perovskite films in detail, the evolution process of organic-inorganic hybrid perovskite films with different annealing conditions is shown in Figure 3. With 0 s annealing, DMF and DMSO solution is not completely volatilized. The contact between the MAI precursor solution (73 mg/mL) and the PbI2 solution belongs to a liquid-liquid diffusion. It is easier for MAI solution to diffuse into the bottom layer, which is conducive to growing flat film. However, part of a solid PbI2 crystal is formed on the topmost layer of the PbI2 film with the annealing condition. With the deposition of MAI precursor solution, loose and uneven perovskite film is partially formed through liquid-solid diffusion (LSD) between precursor solution and the solid topmost layer of PbI2. Therefore, the rough film is obtained, as shown in Figure 3, which is ascribed to the different contact mechanism and crystal growth rate of LLD and LSD between the MAI precursor solution and the PbI2 layer. The adjustment of annealing mainly depends on the time and temperature. Studies have demonstrated that PbI2 film with high crystallinity can be obtained under annealing conditions of high temperature for several minutes, and the MAPbI3 film retains a similar trend. However, in our optimized processing, the compact and flat perovskite film is formed on the liquid PbI2 bottom layer. In the two-step method, the morphology and photophysical properties of the light-absorbing layer can be controlled by the MAI concentration [25]. It is pointed out that the grain size and surface roughness of the perovskite layer are related to the concentration of MAI. In this part of the experiment, different concentrations of MAI are introduced, and the PbI2 layer is not annealed, employing the previous optimization strategy. SEM top views and enlarged views of organic- In the two-step method, the morphology and photophysical properties of the light-absorbing layer can be controlled by the MAI concentration [25]. It is pointed out that the grain size and surface roughness of the perovskite layer are related to the concentration of MAI. In this part of the experiment, different concentrations of MAI are introduced, and the PbI 2 layer is not annealed, employing the previous optimization strategy. SEM top views and enlarged views of organic-inorganic hybrid perovskite films deposited with various concentration of MAI are shown in Figure 4a-f. The compact and smooth grains could be observed from Figure 4a,b, which is similar to the perovskite morphology reported in previous literature [27]; and there are small particles at the boundaries of cubic grains, which may be the residual PbI 2 crystals [30]. Large grain size and decrease in grain boundaries can be observed with the MAI concentration of 73 mg/mL (corresponding to Figure 4b,e). The grain boundaries, as the recombination center of perovskite film, would reduce the device performance. As the concentration of the MAI solution increases to 93 mg/mL, the rough surface of the perovskite film is obtained, which is caused by the large area coverage of the dendritic structure grains and a lot of voids. A gradual process structural transition is demonstrated in Figure 4, indicating that the concentration of MAI precursor solution has a great impact on the growth of perovskite. The dendritic structure grains of Figure 4c are different to other samples significantly, which demonstrates the structural deterioration under excessively high concentrations of MAI.
Crystals 2020, 10, x FOR PEER REVIEW 6 of 12 inorganic hybrid perovskite films deposited with various concentration of MAI are shown in Figure  4a-f. The compact and smooth grains could be observed from Figure 4a,b, which is similar to the perovskite morphology reported in previous literature [27]; and there are small particles at the boundaries of cubic grains, which may be the residual PbI2 crystals [30]. Large grain size and decrease in grain boundaries can be observed with the MAI concentration of 73 mg/mL (corresponding to Figure 4b,e). The grain boundaries, as the recombination center of perovskite film, would reduce the device performance. As the concentration of the MAI solution increases to 93 mg/mL, the rough surface of the perovskite film is obtained, which is caused by the large area coverage of the dendritic structure grains and a lot of voids. A gradual process structural transition is demonstrated in Figure  4, indicating that the concentration of MAI precursor solution has a great impact on the growth of perovskite. The dendritic structure grains of Figure 4c are different to other samples significantly, which demonstrates the structural deterioration under excessively high concentrations of MAI. The significant changes in the surface morphology (size and shape of grains) of perovskite films with different concentrations of MAI could be observed in SEM top views, which may be attributed to the growth state at the interface between the organic-inorganic hybrid perovskite layer and HTL. To explore the influence of the interface on the growth of perovskite, SEM cross-sectional views of light absorption layers prepared with different concentrations of MAI precursor solutions are shown in Figure 5a-c. Some bright spots (corresponding to the yellow circles) at the interface between the perovskite layer and NiOx hole transport layer can be observed in Figure 5a, which may be the PbI2 grains reacting incompletely [31]. A small amount of PbI2 can act as an electron blocking layer, but huge grains may hinder the transport of holes [30]. When the concentration of MAI precursor solution is increased to 73 mg/mL, PbI2 grains no longer exist at the interface, due to the complete reaction of MAI precursor solution and PbI2 solution, which is conducive to transport of charge carrier. In Figure  5c, huge cracks in the perovskite layer and a significant transition of perovskite structure can be observed, indicating the deterioration of the morphology. In addition, the different thickness of perovskite films is observed with the increase in MAI concentration, which can affect not only the XRD peak intensity, but also the absorption and photoluminescence of the films. The significant changes in the surface morphology (size and shape of grains) of perovskite films with different concentrations of MAI could be observed in SEM top views, which may be attributed to the growth state at the interface between the organic-inorganic hybrid perovskite layer and HTL. To explore the influence of the interface on the growth of perovskite, SEM cross-sectional views of light absorption layers prepared with different concentrations of MAI precursor solutions are shown in Figure 5a-c. Some bright spots (corresponding to the yellow circles) at the interface between the perovskite layer and NiO x hole transport layer can be observed in Figure 5a, which may be the PbI 2 grains reacting incompletely [31]. A small amount of PbI 2 can act as an electron blocking layer, but huge grains may hinder the transport of holes [30]. When the concentration of MAI precursor solution is increased to 73 mg/mL, PbI 2 grains no longer exist at the interface, due to the complete reaction of MAI precursor solution and PbI 2 solution, which is conducive to transport of charge carrier. In Figure 5c, huge cracks in the perovskite layer and a significant transition of perovskite structure can be observed, indicating the deterioration of the morphology. In addition, the different thickness of perovskite films is observed with the increase in MAI concentration, which can affect not only the XRD peak intensity, but also the absorption and photoluminescence of the films.
By observing the SEM views, we find that the concentration of MAI precursor solution has a great influence on the surface morphology and structure of the organic-inorganic hybrid perovskite. Figure 6 shows the XRD pattern of perovskite with different concentrations of MAI precursor solution, and the annealing time of PbI 2 is 0 s. The diffraction peaks of (110), (211), and (220), appearing at 2θ = 14.17 • , 23.6 • , and 28.24 • , can be found in the XRD pattern of MAI-53, corresponding to the cubic structure of perovskite shown in Figure 4d. The peak of (001) marked by diamond indicates the residual of PbI 2 , which is consistent with SEM views. The enhanced intensity of the perovskite peaks can be seen from the pattern of MAI-73, which is owing to the increase in grain crystallinity and film thickness. As the concentration increases, the PbI 2 peak disappears, and the splits of (002), (110), (004), and (220) peaks indicate the phase transition to a perfect tetragonal phase, corresponding to the morphology transition to tetragonal structure [31,32]. By observing the SEM views, we find that the concentration of MAI precursor solution has a great influence on the surface morphology and structure of the organic-inorganic hybrid perovskite. Figure 6 shows the XRD pattern of perovskite with different concentrations of MAI precursor solution, and the annealing time of PbI2 is 0 s. The diffraction peaks of (110), (211), and (220), appearing at 2θ = 14.17°, 23.6°, and 28.24°, can be found in the XRD pattern of MAI-53, corresponding to the cubic structure of perovskite shown in Figure 4d. The peak of (001) marked by diamond indicates the residual of PbI2, which is consistent with SEM views. The enhanced intensity of the perovskite peaks can be seen from the pattern of MAI-73, which is owing to the increase in grain crystallinity and film thickness. As the concentration increases, the PbI2 peak disappears, and the splits of (002), (110), (004), and (220) peaks indicate the phase transition to a perfect tetragonal phase, corresponding to the morphology transition to tetragonal structure [31,32]. In our work, the evolution of the organic-inorganic hybrid perovskite structure with the change of MAI concentration is observed. The cubic structure of perovskite is obtained with a low concentration of MAI, and the presence of residual PbI2 at the interface can be found. When the concentration of precursor solution is 73 mg/mL, there is no significant change in perovskite composition. However, the decrease in PbI2 peak proves the higher purity of perovskite formation. The grain size becomes larger and grain boundaries are not obvious, which indicates a transition trend of perovskite structure. With the increase in MAI solution, the growth of dendritic structure delivers the phase transition, deviating the perovskite toward tetragonal structure, which is also proved by the XRD patterns. In addition, there are no peaks of PbI2 (corresponding to ~13°) and MAI (corresponding to ~19°) in the 93-MAI pattern, indicating the pure composition of perovskite, and the  By observing the SEM views, we find that the concentration of MAI precursor solution has a great influence on the surface morphology and structure of the organic-inorganic hybrid perovskite. Figure 6 shows the XRD pattern of perovskite with different concentrations of MAI precursor solution, and the annealing time of PbI2 is 0 s. The diffraction peaks of (110), (211), and (220), appearing at 2θ = 14.17°, 23.6°, and 28.24°, can be found in the XRD pattern of MAI-53, corresponding to the cubic structure of perovskite shown in Figure 4d. The peak of (001) marked by diamond indicates the residual of PbI2, which is consistent with SEM views. The enhanced intensity of the perovskite peaks can be seen from the pattern of MAI-73, which is owing to the increase in grain crystallinity and film thickness. As the concentration increases, the PbI2 peak disappears, and the splits of (002), (110), (004), and (220) peaks indicate the phase transition to a perfect tetragonal phase, corresponding to the morphology transition to tetragonal structure [31,32]. In our work, the evolution of the organic-inorganic hybrid perovskite structure with the change of MAI concentration is observed. The cubic structure of perovskite is obtained with a low concentration of MAI, and the presence of residual PbI2 at the interface can be found. When the concentration of precursor solution is 73 mg/mL, there is no significant change in perovskite composition. However, the decrease in PbI2 peak proves the higher purity of perovskite formation. The grain size becomes larger and grain boundaries are not obvious, which indicates a transition trend of perovskite structure. With the increase in MAI solution, the growth of dendritic structure delivers the phase transition, deviating the perovskite toward tetragonal structure, which is also proved by the XRD patterns. In addition, there are no peaks of PbI2 (corresponding to ~13°) and MAI (corresponding to ~19°) in the 93-MAI pattern, indicating the pure composition of perovskite, and the In our work, the evolution of the organic-inorganic hybrid perovskite structure with the change of MAI concentration is observed. The cubic structure of perovskite is obtained with a low concentration of MAI, and the presence of residual PbI 2 at the interface can be found. When the concentration of precursor solution is 73 mg/mL, there is no significant change in perovskite composition. However, the decrease in PbI 2 peak proves the higher purity of perovskite formation. The grain size becomes larger and grain boundaries are not obvious, which indicates a transition trend of perovskite structure. With the increase in MAI solution, the growth of dendritic structure delivers the phase transition, deviating the perovskite toward tetragonal structure, which is also proved by the XRD patterns. In addition, there are no peaks of PbI 2 (corresponding to~13 • ) and MAI (corresponding to~19 • ) in the 93-MAI pattern, indicating the pure composition of perovskite, and the split of peaks (corresponding to~14 • and 28 • ) shows the perfect tetragonal phase of perovskite. The evolution processes of different samples are shown in Figure 7.  The concentration of MAI also has great impact on the photophysical properties of the perovskite layer, which is reflected in the absorption and photoluminescence. Figure 8 shows the UV-Vis absorption spectra for organic-inorganic hybrid perovskite films with various concentrations of MAI precursor solutions, and the annealing time of PbI2 is 0 s. The strong light absorption of all samples in the range of 450 nm to 750 nm can be observed from Figure 8, indicating the high crystallization quality of films deposited on unannealed PbI2 bottom film. Moreover, the perovskite film of 73-MAI shows the strongest light absorption in the range of 650 nm to 750 nm, which is attributed to the improvement of perovskite crystallinity and increase in film thickness. As the concentration of the precursor solution increases, the red shift of the absorption edge can be observed from 790 nm to 806 nm, indicating the reduction of the band gap. It is speculated that the phase transition of perovskite structure with various concentration results in the narrower band gap of perovskite, which is beneficial to long wavelength absorption [33]. It is worth noting that the enhanced Urbach tail of absorption can be observed with the high degree of MAI concentration (corresponding to the orange circle in Figure 8). The result is similar to previous literature, which is ascribed to structural disorder with high degree of MAI solution [29]. The Urbach energy and steepness parameters are calculated, and listed in Table 1. The concentration of MAI also has great impact on the photophysical properties of the perovskite layer, which is reflected in the absorption and photoluminescence. Figure 8 shows the UV-Vis absorption spectra for organic-inorganic hybrid perovskite films with various concentrations of MAI precursor solutions, and the annealing time of PbI 2 is 0 s. The strong light absorption of all samples in the range of 450 nm to 750 nm can be observed from Figure 8, indicating the high crystallization quality of films deposited on unannealed PbI 2 bottom film. Moreover, the perovskite film of 73-MAI shows the strongest light absorption in the range of 650 nm to 750 nm, which is attributed to the improvement of perovskite crystallinity and increase in film thickness. As the concentration of the precursor solution increases, the red shift of the absorption edge can be observed from 790 nm to 806 nm, indicating the reduction of the band gap. It is speculated that the phase transition of perovskite structure with various concentration results in the narrower band gap of perovskite, which is beneficial to long wavelength absorption [33]. It is worth noting that the enhanced Urbach tail of absorption can be observed with the high degree of MAI concentration (corresponding to the orange circle in Figure 8). The result is similar to previous literature, which is ascribed to structural disorder with high degree of MAI solution [29]. The Urbach energy and steepness parameters are calculated, and listed in Table 1.    Organic-inorganic hybrid perovskite films are prepared on FTO/NiO x substrates to measure the PL property. Figure 9 shows the PL spectra of perovskite films prepared by different concentrations of MAI precursor solution, and the annealing time of PbI 2 is 0 s. It can be seen that the emission peak of MAPbI 3 perovskite is located on around 770 nm. The reason for the high emission peak of sample MAI-53 is the blocking effect of PbI 2 grains on the transport of holes at the interface. The growth of perovskite crystals with moderate concentration of MAI results in less residual PbI 2 crystals and high-flatness perovskite film at the interface, which improves the capability of carrier extraction, and leads to the low emission peak intensity of MAI-73 sample. In addition, the inevitable photon re-absorption may occur in the lager thickness of perovskite film [26]. As the concentration increases, the intensity of the emission peak increases significantly. This abnormal enhancement is due to the phase transition of the perovskite structure. In addition, the full width at half maximum (FWHM) and emission peak center are measured, and listed in Table 2.  The perovskite layer prepared with moderate concentration (73 mg/mL) of precursor solution has a transition trend to tetragonal structure. There is no remnant PbI2 at the interface between the light absorbing layer and hole transport layer. In addition, the annealing time of the PbI2 layer in this part of the experiment is the previously optimized processing time (0 s), ensuring the formed perovskite films are flat. The excellent morphology of perovskite films can be observed. Therefore, the better photophysical properties of the perovskite layer are obtained, which has laid the foundation for the preparation of high-performance perovskite solar cells and photodetectors.  The full width at half maximum (FWHM) and emission peak center of photoluminescence spectra. The perovskite layer prepared with moderate concentration (73 mg/mL) of precursor solution has a transition trend to tetragonal structure. There is no remnant PbI 2 at the interface between the light absorbing layer and hole transport layer. In addition, the annealing time of the PbI 2 layer in this part of the experiment is the previously optimized processing time (0 s), ensuring the formed perovskite films are flat. The excellent morphology of perovskite films can be observed. Therefore, the better photophysical properties of the perovskite layer are obtained, which has laid the foundation for the preparation of high-performance perovskite solar cells and photodetectors.

Conclusions
In summary, the optimization of the preparing process (two-step method) for organic-inorganic hybrid perovskite film was investigated in our work. Firstly, the effect of PbI 2 annealing time on the film flatness of the perovskite was investigated. The deposition of MAI solution through liquid-liquid diffusion was more conducive to growing high-flatness perovskite film. In addition, various MAI concentrations were introduced to the preparation of the perovskite film. The enhanced absorption and carrier extraction capability of perovskite film were obtained with moderate MAI (73 mg/mL). A high degree of MAI concentration led to the transition of perovskite to typical tetragonal structure, resulting in the deterioration of film morphology.
The suitable annealing time of PbI 2 and concentration of MAI were determined in our experiments. Moreover, the optimization process for controlling the morphology and structure of perovskite was investigated. These results provide novel ideas to modulate the growth of MAPbI 3 crystal under the two-step method.
For the preparation of the inverted device, we just made a preliminary attempt by using processing techniques for the perovskite absorption layer. We will apply the optimization process for perovskite layer to the fabrication of device, and optimize the overall device to improve the power conversion efficiency.